Eﬀects of TiO capping layer on reset current 2
Eﬀects of TiO2 capping layer on reset current of lateral phase change memory 145 Eﬀects of TiO2 capping layer on reset current of lateral phase change memory Santipab Sainon1 and Chiranut Sa-ngiamsak2 , Non-members ABSTRACT Lateral Phase Change Memories (LPCMs) gained a lot of interesting due to its simpler fabrication process and lower reset current comparing with verticalstructure phase change memories. The capping layer can be easily fabricated and changed on the active phase-change region of LPCM. The knowledge of capping layer on the thermal generation and diﬀusion on LPCM can provide an alternative design approach to alleviate the high reset current issue of PCM. The location and thickness of TiO2 capping layer were studied in order to achieve higher power consumption eﬃciency using ﬁnite element analysis. The four LPCM structures with various location of capping layer were modelled. The simulation results found that addition of TiO2 capping layer can increase power eﬃciency. The suitable location to place TiO2 capping layer is at the centre of the active phase-change layer found in Model 4. The thickness of capping layer was developed based on Model 4; and thickness of 40nm was given the best result. The combination of proper location and thickness of TiO2 capping layer can oﬀer a reduction of the LPCM reset current by 24%. Keywords: Phase Change Memory, LPCM, Reset Current, Finite Element, Structure Design, TiO2 Capping Layer, Capping Layer Location, Capping Layer Thickness 1. INTRODUCTION Nowadays, there are the continuously increasing of functionalities and performances of consumer electronic products that are supporting the growing demand for non-volatile memories (NVM) [1,2]. Currently, the most popular NVM is ﬂash memory. Nevertheless, Flash memory is facing severe scalability limitations [3, 4]. New memories have been explored for the next generation NVMs technologies. Phase change memory (PCM) is considered as one of the most promising candidate for next generation NVM Manuscript received on January 24, 2014 ; revised on July 22, 2014. Final manuscript received September 17, 2014. 1,2 The authors are Department of Electrical Engineering, Khon Kaen University, Khon Kaen, 40002, Thailand., Email: [email protected] and [email protected] 2 The author is with Department of Electrical Engineering and Sustainable Infrastructure Research and Development Center, Khon Kaen University, Khon Kaen, 40002, Thailand., E-mail: [email protected] 2 Corresponding Author technology due to its low power consumption, high scalability, high read/write speeds, long cycle life and good compatibility with standard complementary metal oxide semiconductor (CMOS) processing [5-7]. The PCM cell is stored data by switching the structure of a phase change material, chalcogenide material, typically Ge2 Sb2 Te5 (GST), which can be reversibly switched between the amorphous (high resistivity) and the crystalline (low resistivity) state by Joule heating due to current ﬂow. High reset current is needed to switch the phase change material from the crystalline state to amorphous state (the reset operation). It has become the major barrier for the further scaling of PCM devices. Therefore, reducing the reset current is important issue to reach both high density and low power consumption. Approaches on material design and property can reduce the reset current such as doping with O ,Si, N and other elements. The other eﬀective method is to work on the structural design of PCMs. There are several proposed new structure for vertical PCM structure such as edge contact PCM device  and µ-trench architecture . Nevertheless, the complication on device fabrication has become the drawback of those complicated structures. Recently, Lateral phase change memories have gained a lot of interesting due to its simpler fabrication process, easier integration with complementary metal-oxide semiconductor (CMOS) and lower reset current comparing with vertical PCM structure [13-15]. Thus, LPCMs have gained lots of attention particularly on its physical mechanisms. Castro et al. studies the thermoelectric Thomson eﬀect of the diﬀerent LPCM, such as ﬁne line cell, dog-bone cell and T-cell . Kim et al. presented a mechanism of the electrical switching due to electro-migration effect . Moreover, another approach on additional capping layer, which can be easily fabricated and deposited on the active region of phase change layer have been explored [19-21]. The understanding the eﬀect of capping layer on the thermal generation and diﬀusion in LPCM is an important issue to design a low reset current LPCM structure; particularly on the type of material, structure, location, and the thickness of capping layer. In this paper, the location and thickness of TiO2 capping layer were studied in order to achieve higher power consumption eﬃciency using ﬁnite element analysis. The four LPCM structures with various location of capping layer were modelled and studied its 146 ECTI TRANSACTIONS ON COMPUTER AND INFORMATION TECHNOLOGY VOL.8, NO.2 November 2014 thermal eﬃciency. Later on, the thickness TiO2 capping layer on power consumption eﬃciency was investigated. Finally, the eﬃciency of the LPCM with and without TiO2 capping layer was compared. reset process, a drastic resistance variation of PCMs is attributed to phase-change triggered by Joule heating. The electrical current ﬂows through the LPCM cell, then the heat is generated within LPCM device by Joule heating, which can be expressed as, 2. MODELLING AND SIMULATIONS LPCM structure with and without TiO2 capping layer of 90 nm were depicted. Three locations of placed capping layers were investigated at the edge, 1 /4 and 1 /2 of contact spacing and the LPCM structure without a capping later was used as a reference as Model 1 while the rest were LPCM structure with TiO2 capping layer of 90 nm at three various locations were labeled as Model 2, 3 and 4. The simulation was carried out using physics-based and Finite Element Simulation (FEM) Program, COMSOL Multiphysicsr. 2. 1 LPCM Structure LPCM cell geometry of 90nm node technology was considered and shown in Fig.1 (a). It comprises of 100 nm SiO2 -ZnS ﬁlm thickness, 30 nm, phase change material (Ge2 Sb2 Te5 , GST), and two electrode contacts (titanium nitride, TiN) with thickness of 100 nm. The cell was enclosed by electrical insulating material (silicon dioxide, SiO2 ). Figure 1(b) displayed LPCM with 20 nm TiO2 capping layer. The location of the TiO2 layer is deﬁned by d. Three conditions are investigated in the subsequent analysis: Model 2 (d = 0 nm); Model 3(d = 90nm); and Model 4 (d = 180 nm). Fig.1: LPCM model geometry (a) The reference model (Model 1) and (b) The LPCM with capping layer at various locations (Model 2-4). 2. 2 Electro-Thermal Modeling The temperature proﬁle and current distribution inside the LPCM device were examined. The numerical models were established in the three dimensional (3D) ﬁnite element method (FEM) analysis on the basis of the electrical-thermal interaction. During the Q = ρ|J|2 (1) where Q is the Joule heat induced by current pulse, ρ is the electric resistivity, J is the electric current density and V is the electric potential. The temperature distribution caused by heat transfer in the device can be obtained by solving the heat conduction equation as following: dC ∂T − ∇ · (k∇T ) = Q ∂t (2) where d is the density, T is the temperature, C is the volumetric heat capacity, k is the thermal conductivity and t is the time. The equations (1) and (2) are coupled with Laplace equation: ∇(σ · ∇V ) = 0 (3) where σ is the electric conductivity and V is the electric potential. ∂2T ∂2T ∂2T 1 ∂T + + = 2 2 2 ∂x ∂y ∂z D ∂t (4) k Where D = ρ.c is thermal diﬀusivity and constant p k, ρ and cp are thermal conductivity, density, and speciﬁc heat of the materials. The assumptions for this work are: (a) all of the exterior boundaries were set at room temperature (300K) whereas those of interior boundaries were continuous boundary conditions (b) all of the electrical boundary was set to electrical insulation expect for one boundary of the right electrode set to ground and one boundary of the left electrode where an electrical current pulse was applied to LPCM cell and (c) the material properties used in this study are presented in Table I. These parameters remain constant throughout during calculations. Table 1: Physical properties of materials used for the simulations. Material GST TiN TiO2 SiO2 ZnSSiO2 Mass density d(kg/m2 ) 6200a Specific heat cp (J/kgK) 202a Thermal conductivity k(W/mK) 0.46a Electrical resistivity ρ(Ωm) 3.6×10−4a 5240b 4230e 2330a 784b 711e 730a 3650d 560d 22b 0.25c 1.4a 0.21d 1×1017d a Ref.  b Ref.  c Ref.  d Ref.  e Ref.  1×10−6b 1×10−2d 1×1014a Eﬀects of TiO2 capping layer on reset current of lateral phase change memory 147 The temperature caused by Joule heating along y-axis of 4 models was monitored and plotted in Fig.2(a) while the temperature proﬁle around the active area were displayed in Fig.2(b)-Fig.2(e). 3. RESULTS AND DISCUSSIONS The results were classiﬁed into two eﬀects of TiO2 chapping layer: Location and Thickness with some discussion on the results. 3. 1 Location eﬀect of TiO2 capping layer on the thermal eﬃciency Fig.2: (a)Peak temperature caused by Joule heating along y-axis (b)-(e) Temperature proﬁle of LPCM cells (Model 1-4) in the cross-section top view(y-axis) with a 104uA and 30 ns current pulse. The analysis of LPCM heating eﬃciency during the reset process through the temperature distribution is very important in order to gain a deep understanding of the LPCM cell operation. The switching of PCM cell to a high-resistance amorphous or reset state requires temperature at the active region beyond melting point (900K). The molten region is an eﬀective programming area which overlaps the entire active region of phase-change layer. This area deﬁned a completion of reset operation. The location of TiO2 capping layer targeted to reset current reduction was obtained by performing transient simulation with the same current pulse as shown in Fig 2. Fig.2 shows the temperature proﬁle in each model in the cross-section top view (along yaxis) after applying a current pulse with amplitude of 104 uA and 30 ns pulse width. The comparison of temperature proﬁle shown in Fig.2(b)-Fig.2(e) indicated the proper location to place TiO2 capping layer on the eﬀective programming. Fig.2(a) reveals the maximum temperature of all 4 models. It concludes the proper location of TiO2 capping layer is at the centre of two contacts (Model 4) which provides the best results comparing with other places. Moreover, the results in Fig.2 display the eﬀective programming area of LPCM with TiO2 capping layer is wider than that LPCM without capping layer and smaller when the TiO2 capping layer is located away from the center active region due to the thermal conductivity of TiO2 (0.25W/mK) is lower than SiO2 (1.4W/mK). The additional TiO2 capping layer on a simple LPCM prevents heat diﬀusion mechanism at an active phase-change region of LPCM. Then, the active GST cell under TiO2 capping layer is the peak temperature. Apart from the temperature caused by Joule heating at the active area should be higher than the melting point temperature of GST material (900K), the completion of active area is able to identify by the boundary of temperature contour of molten as shown in Fig.3. The melting point temperature of GST (900K) was considered as the boundary of cell completion during the reset state. The veriﬁcation of the cell completion of those four models were carried out by applying the same reset current pattern of 104uA 148 ECTI TRANSACTIONS ON COMPUTER AND INFORMATION TECHNOLOGY VOL.8, NO.2 November 2014 and 30 ns pulse width to the LPCM with and without capping layer FEM models. capping layer performs well at the centre area due to its location is the longest distance to TiN contact acting as a heat sink. Regarding the completion of the active cell during the reset state, the conclusion can be drawn from Fig.3(b)- Fig.3(e). Temperature contour was plotted and the boundary of cell completion was observed using 900K contour line. Model 1 (the reference) and Model 2 show the incompletion of the active GST cell during the reset state with the 104uA and 30 ns current pulse width while the 900K contour line of Model 3 and Model 4 cover the whole GST active area which identify the completion of the reset state. The completion of an active GST area during the reset state reﬂects the memory cell stability and its retention time. 3. 2 Thickness eﬀect of the TiO2 capping layer on power consumption eﬃciency The proper location of TiO2 capping layer was identiﬁed at the centre of the TiN contacts due to the results shown in the previous section. Further reset current reduction was carried out through the study of thickness eﬀect of TiO2 capping lay on the power consumption eﬃciency. The optimum thickness was deﬁned as the layer thickness providing the minimum reset current with cell completion during the reset state. The thickness of TiO2 layer was varied from 0nm - 80nm with 90nm node technology. The minimum reset current amplitude with cell completion during the reset state was noted at various thickness of TiO2 . The reduction of current amplitude was plotted in percentage using Model 1 as a reference as both results shown in Fig.4. Fig.3: (a) Peak temperature along x-axis at the effective programming area of each LPCM model with 104uA, 30ns current pulse. (b)-(e) Temperature contour at cross-section view (along x-axis) of Model 14. The explanation of the proper location of TiO2 capping layer at the centre between two TiN contacts can be described through the material thermal conductivity. The thermal conductivity of TiN, SiO2 , and TiO2 are 22W/mK, 1.4W/mK, and 0.25W/mK. The highest thermal conductivity is TiN contact; hence, TiN contacts act as a heat sink as well. The main purpose of adding TiO2 layer is to prevent heat loss over the active GST area in order to increase the temperature and also widening the active cell or the completion of active cell during the reset state. TiO2 Fig.4: Reset current as a function of the TiO2 thickness after applying a 30ns pulse (left). % Reduction of reset current as a function of the TiO2 thickness after applying a 30ns pulse (right). Fig.4 illustrates the reduction in percentage of a reset current as a function of the TiO2 thickness after Eﬀects of TiO2 capping layer on reset current of lateral phase change memory 149 applying a 30 ns pulse (right) while the reset current of LPCM without TiO2 capping layer was used as a reference. It indicated that the additional TiO2 capping layer can oﬀer a reduction of the LPCM reset current by 24% with the optimised TiO2 thickness of 40nm. The reset current signiﬁcantly decrease with the increase of TiO2 thickness in the range of 0-40 nm due to the TiO2 (0.25W/mK) has lower thermal conductivity than SiO2 (1.4W/mK). Therefore, the increment of TiO2 thickness leads to higher thermal resistance of TiO2 , which help to resist the heat transfer to SiO2 area during the reset state. On the other word, heat loss at the active GST area was reduced; therefore, lower reset current was required to achieve the reset state with completion when the thickness of TiO2 capping layer increases from none to 40 nm. However, the reset current was saturated with TiO2 thickness over 40 nm due to the relative large heat leakage into the material is caused by the relative large heat diﬀusion length of material (Λ) [15,16]. Heat diﬀusion length of material (Λ) can be described as: Λ= √ D∆t (5) √ Λ = D∆t ∼ = 50nm, where D = kT iO2 /CT iO2 is thermal diﬀusion constant of TiO2 material, kT iO2 is thermal conductivity of TiO2 , CT iO2 is the heat capacity of TiO2 and ∆t = 30ns is the duration of the constant current pulse. Fig.6: Temperature proﬁle at the eﬀective programming area of LPCM cells in the cross-section side view (along x-axis) with 100uA, 30ns reset current pulse,(a) LPCM without TiO2 capping layer,(b) LPCM with a TiO2 capping layer thickness of 40nm. (c) Temperature along x-axis of LPMC without TiO2 and with optimised TiO2 capping layer. Fig.5: Geometry in z-axis of LPCM with TiO2 capping layer. Considering the z-axis, GST thickness is 30nm and TiO2 thickness is d = 40nm, the distance from the centre of GST material to the edge of TiO2 boundary is 55nm (15nm of GST and 40nm of TiO2 ) which is the limit of diﬀusion length of material as calculated in Eq(5). Beyond 40nm, the increment of TiO2 thickness has played no signiﬁcance in reset current reduction due to diﬀusion length of material limitation; hence the optimize TiO2 thickness is 40nm for TiO2 with the reset current of ∆t = 30ns. Figure 6(a-b) illustrate the comparison of the temperature proﬁle of LPCM with and without TiO2 capping layer. It clearly validates the beneﬁt of adding TiO2 capping layer into a simply LPCM structure for the purpose of reset current reduction. Fig.6(c) provides another point of view to display the incompletion of memory cell for the case of LPCM without TiO2 capping layer. Fig.7 demonstrates the maximum temperature at the active phase-change region of the LPCM without TiO2 capping layer and with 40nm TiO2 capping layer. Temperature rises continuously before becoming saturated during the “on-current” period; and then drop drastically during the “oﬀ-current” period. This shows a fast temperature ramping up and down of the LPCM with 40 nm TiO2 capping layer cell. The the simulation results clearly reveal the maximum temperature of LPCM with 40 nm TiO2 capping layer cell is approximately 1.2 times higher than the case of the LPCM without a TiO2 capping layer. 150 ECTI TRANSACTIONS ON COMPUTER AND INFORMATION TECHNOLOGY VOL.8, NO.2 November 2014     Fig.7: Maximum temperature proﬁles for LPCM cell at position in active region with reset current pulse of 100uA and 30ns on current.  4. CONCLUSION  The simulation results of this work conclude that: (a) Addition of TiO2 capping layer in LPCM can reduce power consumption during data recording (b) The proper location of TiO2 capping layer is at the centre of the active phase-change layer (c) The optimised TiO2 capping layer with 40 nm thickness can oﬀer a reduction of the LPCM reset current by 24% This signiﬁes a superior performance of the LPCM with 40 nm TiO2 capping layer cell over a simple LPCM without a TiO2 capping layer. 5. ACKNOWLEDGEMENT This work is endorsed by Western Digital (Thailand) Company Limited and ﬁnancially supported by National Electronics and Computer Technology Centre (NECTEC), National Science and Technology Development Agency (NSTDA) Thailand and Data Storage Technology and Applications, King Mongkut’s Institute of Technology Ladkrabang Thailand (HDD-03-52-10M).      References     Geoﬀrey W. and et al., “Phase change memory technology,” Journal of Vacuum Science and Technology B, Vol. 28, pp. 223-262,2010. W. Brown and J. Brewer, “Non-volatile Semiconductor Memory Technology”, IEEE press, New York, 1998. Roberto B., and Pirovano A., “Non-volatile Memory Technologies: Emerging Concepts and New Materials,” Material Science in Semiconductor Processing, Vol. 7,pp. 349-355,2004. Yoshihisa Fujisaki, “Current Status of Nonvolatile Semiconductor Memory Technology,”   Japanese Journal of Applied Physics, Vol. 49,2010. S. Lai, “Current status of the phase change memory and its future,” in IEDM Tech. Dig., pp. 255258, 2003. R.Y. Kim, H.G. Kim and S.G. Yoon, “Structural properties of Ge2 Sb2 Te5 thin ﬁlms by metal organic chemical vapor deposition for phase change memory applications,” Appl.Phys.Lett,Vol.89, pp.102107-102109,2006. S.R. Ovshinsky, “Reversible electrical switching phenomena in disordered structures,” Phys. Rev. Lett., Vol. 21, pp.1450-1453, 1968. N. Matsuzaki and et al.,“Oxygen-doped GeSbTe phase-change memory cells featuring 1.5V/100uA standard 0.13-um CMOS operations,” IEDM Tech. Dig., 2005. Feng. J. and et al., “Si Doping in Ge2Sb2Te5 Film to Reduce the Writing Current of Phase Change Memory”, Applied Physic A: Materials Science & Processing, Vol.87, pp.57-62, 2007. M. Kim, and et al., “Electrical Switching Characteristics of Nitrogen Doped Ge2Sb2Te5 Based Phase Change Random Access Memory Cell,” Solid State Phenomena, Vol.21, pp.124-126, 2007. H. Ha et al., “An edge contact type cell for phase change RAM featuring very low power consumption,” Proc. Symp. Very Large Scale Integr. (VLSI) Technol., pp 175-176, 2003. F. Pellizzer and et al., “Novel u-trench phase change memory cell for embedded and standalone non-volatile memory applications”, Proc. Symp. Very Large Scale Integr. (VLSI) Technol., pp 18-19, 2004. You Yin, Hayato Sone, Sumio Hosaka, “Lateral SbTeN based multi-layer phase change memory for multi-state storage,” Microelectronic Engineering, Vol. 84, pp 2901-2906, 2007. R. L. Martijn, W. S. M. M. K, Bas, and R. A. M. Wolters, “Low-cost and nanoscale non-volatile memory concept for future silicon chips,” Nat. Mater., Vol.4, pp.347,2005. F. J. Jedema, M. A. A in’t Zandt, and W. S. M. M Ketelaars, “Program window of doped Sb2Te phase change line cells,” Appl. Phys Lett., Vol. 9, pp 203-509, 2007. Jedema, F.J.; ’t Zandt, M.A.A.; Wolters, R.A.M.; Castro, D.T.; Hurkx, G.A.M.; Delhougne, R., “Scaling Properties of Doped Sb2Te Phase Change Line Cells,” Non-Volatile Semiconductor Memory Workshop, 2008 and 2008 International Conference on Memory Technology and Design. NVSMW/ICMTD 2008. Joint , vol., no., pp.43,45, 18-22 May 2008. D. T. Castro and et al., “Evidence of the Thermo-Electric Thomson Eﬀect and Inﬂuence on the Program Conditions and Cell Opti- Eﬀects of TiO2 capping layer on reset current of lateral phase change memory          mization in Phase-Change Memory Cells,” Proceedings of the IEEE Electron Devices Meeting (IEEE, New York, 2007), pp. 315-318. C. Kim, D. Kang, T. -Y. Lee, K. H. P. Kim, Y. -S. Kang, J. Lee, S. -W. Nam, K. -B. Kim, and Y. Khang, “Direct evidence of phase separation in Ge2 Sb2 Te5 in phase change memory devices,” Appl. Phys. Lett., Vol.94, pp 193504 , 2009. N. Ohshima, “Crystallization of germaniumantimony-tellurium amorphous thin ﬁlm sandwiched between various dielectric protective ﬁlms,” J. Appl. Phys., Vol. 79, pp 8357,1996. Young Sam Park, Sang Ouk Ryu, Kyu Jeong Choi, Seung Yun Lee, Sung Min Yoon, and Byoung Gon Yu,“Stress reduction during phase change in Ge2 Sb2 Te5 by capping TiN ﬁlm,” Materials Transactions, J Mater Sci: Mater Electron, Vol.18 ,pp 1079-1082, 2007. Young Sam Park, Jung Wook Lim, Woo Seok Yang, Seung-Yun Lee, Sung-Min Yoon, and Byoung Gon Yu,“Stress Reduction of Ge2Sb2Te5 by Inhibiting Oxygen Diﬀusion,” Materials Transactions, Vol. 49, No. 9, pp. 2107 to 2111, 2008. You Yin and Sumio Hosaka, “Low-ResetCurrent Ring-Conﬁned-Chalcogenide Phase Change Memory,” Jpn. J. Appl. Phys., Vol. 51, pp.104202, 2012. D.H. Kang and et al., “An experimental investigation on the switching reliability of a phase change memory device with an oxidized TiN electrode,” J. Appl. Phys.,Vol. 100, pp.054506054508, 2006. X. Cheng, S. Zhitang, L. Bo, F. Songlin and C. Bomy, “Lower current operation of phase change memory cell with a thin TiO2 layer,” Appl. Phys. Lett., Vol. 92, pp.062103-062105, 2008. D. Ristau and J. Ebert, “Development of a thermographic laser calorimeter,” Appl. Opt.,Vol. 25, pp.4571-4578, 1986. MatWeb’s Services Available to the Materials Community [Online]. Available: http://www.matweb.com/ [Accessed: 20 June 2014]. Chiranut Sa-ngiamsak received B.Eng in Electrical Engineering from Khon Kaen University, Khon Kaen, Thailand, M.Phil in Electrical Engineering from The University of Manchester, England, and Ph.D in Electrical Engineering and Electronics from University of Manchester Institute of Science and Technology (UMIST), England in 1994, 1998, and 2004, respectively. Since 1994, she has become a full-time lecturer at Department of Electrical Engineering, Faculty of Engineering, Khon Kaen University, Thailand where she is now holding an assistant professorship. Her research interests are High Speed 151 Solid State Device and Memory Technology. She is now actively working on failure analysis of memory technology and solid-state semiconductor design. Santipap Sainon received B.Eng in Electrical Engineering from Khon Kaen University, Khon Kaen, Thailand in 2008 and right now he is now pursuing his master degree in Electrical Engineering at Khon Kaen University under the supervision of Asst.Prof.Chiranut Sa-ngiamsak. His research interests are Phase Change Memory and Hybrid Drive.